efflorescence brings out salts that are not ordinarily part of the cement stone, it is not a structural, but, rather, an aesthetic concern. For controlling primary efflorescence, formulations containing liquid fatty acid mixtures (e.g., oleic acid and linoleic acid) have commonly been used. The oily liquid admixture is introduced into the batch mix at an early stage by coating onto the sand particles prior to the introduction of any mix water, so that the oily admixture is distributed uniformly throughout the concrete batch mix. Secondary efflorescence Secondary efflorescence is named such as it does not occur as a result of the forming of the cement stone or its accompanying hydration products. Rather, it is usually due to the external influence of concrete poisons, such as chlorides. A very common example of where secondary efflorescence occurs is steel-reinforced concrete bridges as well as parking garages. Saline solutions are formed due to the presence of road salt in the winter. This saline solution is absorbed into the concrete, where it can begin to dissolve cement stone, which is of primary structural importance. Virtual stalactites can be formed in some cases as a result of dissolved cement stone, hanging off cracks in concrete structures. Where this process has taken hold, the structural integrity of a concrete element is at risk. This is a common traffic infrastructure and building maintenance concern. Secondary efflorescence is akin to osteoporosis of the concrete. For controlling secondary efflorescence, admixtures containing aqueous-based calcium stearate dispersion (CSD) are often added at a later stage of the batching process with the mix water. In a typical batching process, sand is first charged into the mixer, then the oil-based primary anti-efflorescence admixture is added with constant mixing to allow the oil to coat the sand. Then coarse aggregates, colorants, and cement are added, followed by water. If CSD is used, it is then introduced usually at this point during or after the addition of the mix water. CSD is an aqueous dispersion wherein fine solid particles of calcium stearate are suspended in the water uniformly. Commercially available CSD has an average particle size of about 1 to 10 micrometres. The uniform distribution of CSD in the mix may render the resulting concrete masonry unit water repellent, as CSD particles are well distributed in the pores of the unit to interfere with the capillary movement of water. Calthemite is also a secondary deposit